Arabian Journal of Chemistry (2016) 9, 121–135
King Saud University
Arabian Journal of Chemistry
Synthesis, characterization and corrosion inhibition
efficiency of N-(4-(Morpholinomethyl Carbamoyl
Phenyl) Furan-2-Carboxamide for brass in HCl
* Corresponding author. Tel.: +91 9500921100.
E-mail address: firstname.lastname@example.org (N. Zulfareen).
Peer review under responsibility of King Saud University.
Production and hosting by Elsevier
1878-5352 � 2015 The Authors. Production and hosting by Elsevier B.V. on behalf of King Saud University.
This is an open access article under the CC BY-NC-ND license (http://creativecommons.org/licenses/by-nc-nd/4.0/).
N. Zulfareen *, K. Kannan, T. Venugopal, S. Gnanavel
Department of Chemistry, Government College of Engineering, Salem 636011, India
Received 8 April 2015; accepted 19 August 2015
Available online 31 August 2015
Abstract A mannich base namely N-(4-(Morpholinomethyl Carbamoyl Phenyl) Furan-2-
Carboxamide (MFC) was synthesized and characterized by FT-IR, 1H NMR, and 13C NMR.
The molecular weight of MFC was confirmed by LC-MS. The inhibition effect of MFC on brass
in 1 M HCl medium has been investigated by weight loss measurement, potentiodynamic polariza-
tion, electrochemical impedance spectroscopy (EIS) and cyclic voltametry (CV). Thermodynamic
parameters such as free energy, entropy and enthalpy were calculated to describe the mechanism
of corrosion inhibitor. The inhibition efficiency of MFC increases with increase in concentration
and temperature ranges from 30 �C to 60 �C. Polarization measurements indicated that MFC acts
as a mixed type corrosion inhibitor. AC impedance indicates that Rct value increases with increase
in the concentration of inhibitor. CV reveals that the oxidation of the copper is controlled by the
addition of inhibitor on the brass metal. Surface analysis using scanning electron microscope
(SEM) shows a significant morphological improvement on the brass surface with the addition of
the inhibitor. The adsorption of MFC on brass obeys Langmuir adsorption isotherm. The molec-
ular structure of MFC was distorted to quantum chemical indices using density functional theory
(DFT) which indicates that the inhibition efficiency of MFC is closely related to quantum param-
� 2015 The Authors. Production and hosting by Elsevier B.V. on behalf of King Saud University. This is
an open access article under theCCBY-NC-ND license (http://creativecommons.org/licenses/by-nc-nd/4.0/).
Brass is an alloy of copper and zinc used in industries for the
functional and esthetic purpose. Brass is extensively used in
manufacturing applications such as domestic water
distribution system inside the valves, heat exchangers, cooling
water systems, power generation plants, petrochemical heat
122 N. Zulfareen et al.
exchangers, plumb fittings and plumbing fixtures due to its
excellent electrical and thermal conductivity (Al-Mobarak
et al., 2010; Fouda and Wahed, 2011; Bastidas et al., 2003).
Brass is corrosion resistance to the atmosphere and chemical
agents owing to its mechanical property. But its corrosion is
a universal environmental problem, and it affects all aspects
of industries. The increasing interest in the manufacture and
use of hydrochloric acid in industries and industrial water sup-
ply has created the need for corrosion resistance of brass in this
acid (Benabdellah et al., 2011a,b).
Corrosion is the major problem for industrial water supply
and circulation system. Protection against corrosion was car-
ried out by adding inhibitors in acidic medium. These inhibi-
tors are organic compounds containing heteroatoms with
high electron density such as Nitrogen, Oxygen, Sulfur, Phos-
phorous and aromatic rings that cause adsorption on the metal
surface (Ramji et al., 2008). The action of the inhibitor is elec-
trochemical and involves the discharge of positively charged
particles at the cathodic area that forms an adsorbed layer
on the metal surface. The adsorption of inhibitor takes place
depends on their physical and chemical properties, the nature
of metal and the type of electrolyte solution.
Nowadays Mannich base compounds have been of interest
in order to obtain efficient corrosion inhibitors since they pro-
vide much greater inhibition efficiency compared to corre-
sponding amines and aldehydes. Mannich reactions consist
of an amino alkylation of an acid proton placed next to a car-
bonyl functional group with formaldehyde and ammonia or
any primary or secondary amine (Chaluvaraju and Bhat,
2010). The final product is a b-amino-carbonyl compound also
known as a mannich base. Tertiary amines are not used due to
the lack of NAH proton to form the intermediate imine.
The present paper reports on the anticorrosive behavior of
N-(4-(Morpholinomethyl Carbamoyl Phenyl) Furan-2-
Carboxamide) (MFC) a mannich base for brass in hydrochlo-
ric acid solution. Inhibition efficiency of the Mannich base on
brass was studied using Electrochemical impedance spec-
troscopy (EIS), potentiodynamic polarization methods and
weight loss method. Further SEM analysis was studied to
determine the surface coverage. Cyclic voltammetry was used
to study the behavior of the alloy in the oxidation and reduc-
tion potential. Density functional theory (DFT) was used to
correlate the inhibition with the coefficients of molecular orbi-
tal such as highest occupied molecular orbital (HOMO) and
Lowest occupied molecular orbital (LUMO). The energy dif-
ference between EHOMO and ELUMO, atomic charges and
dipole moment of the synthesized mannich base was also stud-
ied for the theoretical prediction of the corrosion inhibition
2.1. Synthesis of CFC
N-(4-Carbamoylphenyl)Furan-2-Carboxamide (CFC) was
prepared by a procedure similar to the method reported in
the literature (Jumade et al., 2009). 4 -Amino benzamide
(3.00 g, 0.0220 mol) and 2-furoyl chloride (3.428 g,
0.0264 mol) were dissolved in mixture of MDC (70 ml) and
THF (25 ml). Triethylamine (7.77 g) was added, and the mix-
ture was stirred in the presence of nitrogen atmosphere for
24 h. The reaction mixture was washed with water, filtered
and dried over high vacuum pump. The CFC was character-
ized by spectral techniques such as FT-IR, NMR, and LC-
MS. Fig. 1 represents the synthesis of CFC.
2.2. Characterization of CFC
Yield 93%, white solid, m.p.186–190 �C., IR (KBr, mmax
cm�1; 3387, 3179 (NH, St, Amide), 1658 (C‚O), 1617 (NH,
Bend, Amide), 1400 (CN, Amide), 1474, 1527 (C‚C), 1179
(CAO, furan), 841 (CH, Ar, oop). 1H NMR (400 MHz,
DMSO-d6) d(ppm): 6.71(1H, Furan), 7.36 (1H, furan), 7.80–
7.84 (4H), 7.85–7.87 (2H, Amide), 7.95 (1H, furan), 10.36
(1H, Amide). 13C NMR (400 MHz, DMSO-d6) d(ppm): d
112.1, 115.0, 119.2, 128.1, 129.1, 141.1, 145.0, 147.2, 156.2
(C‚O), 167.3 (C‚O). MS (EI): m/z (%) = 231.
Figs. 2a, 2b, 2c, 2d represent the FT-IR, 13C, 1H and LC-
MS of CFC respectively.
2.3. Synthesis of MFC
The mixture of CFC (0.0130 mol, 3 g), morpholine
(0.0130 mol, 1.1363 g), and formaldehyde (0.01956 mol,
0.587 g) was dissolved in ethanol. The reaction mixture was
refluxed for 48 h at 80 �C. The white solid obtained was fil-
tered, washed with cold ethanol and followed by petroleum
ether. The resulted mass is dried and recrystallized from etha-
nol (Nagham et al., 2013; Karthik et al., 2011). The MFC was
characterized by spectral techniques such as FT-IR, NMR,
and LC-MS. Fig. 3 represents the synthesis of MFC.
2.4. Characterization of MFC
Yield 90%, white Solid, m.p.176–180 �C., IR (KBr, mmax
cm�1; 3305 (NH), 3177 (CH, Ar), 2958, 2843 (CH, Aliph),
1666 (C‚O), 1646 (NH, bend), 1548, 1472 (C‚C), 1304
(CAN, amide), 1183 (CAO, furan) 1115 (CAO, morpholine),
1023 (CAN, Amine), 852 (CH, Ar, oop). 1H NMR
(400 MHz, DMSO-d6) d(ppm): 2.50 (4H), 3.55 (4H), 4.15
(2H), 6.72 (1H, furan), 7.39 (1H, furan), 7.83–7.89 (4H), 7.96
(1H, furan), 8.72(1H, Amide), 10.40 (1H, Amide). 13C NMR
(400 MHz, DMSO-d6) d(ppm): h 50.62, 61.23, 66.5, 112.7,
115.6, 119.9, 128.7, 129.6, 141.7, 146.4, 147.7, 156.8 (C‚O),
166.9 (C‚O). MS (EI): m/z (%) = 329.87.
Figs. 3a, 3b, 3c, 3d represent the FT-IR, 13C, 1H and LC-
MS of MFC respectively.
The solubility of MFC was found to be 0.5 g in 100 ml of 1 M
HCl. The standard solution of 1 M hydrochloric acid was pre-
pared using double distilled water. The experiments were car-
ried out in the presence and absence of MFC at various
concentration ranges from 0.3 mM to 2.1 mM, and tempera-
ture ranges from 30 �C to 60 �C.
Brass with the composition of Cu (60.66%), Zn (36.58%), Sn
(1.02%) and Fe (1.74%) was used and exposed geometrical